Chapter 2Battery CathodesMarca M. DoeffGlossaryAnode – (negative electrode) This electrode donates electrons during cell discharge.Battery A device consisting of one or many electrochemi- cal cells connected together, in which chemical energy is converted into power. These can be fur- ther categorized as primary (non-rechargeable) or secondary (rechargeable) systems.Capacity The amount of charge that a battery contains, often expressed as mAh or Ah. This depends on the size of the battery and its chemistry. Rated capacity also depends on the current used.Cathode – (positive This electrode accepts electrons during cellelectrode) discharge.Cell One unit of a battery, commonly consisting of an anode, a cathode, an electrolyte, a separator, and two current collectors.Energy density Energy per unit volume or weight of a material oror speciﬁc energy a device, respectively, often expressed as Wh/L or Wh/kg. Energy is a product of the cell voltage and capacity per unit volume or weight.This chapter was originally published as part of the Encyclopedia of Sustainability Scienceand Technology edited by Robert A. Meyers. DOI:10.1007/978-1-4419-0851-3M.M. Doeff (*)Environmental Energy Technologies Division, Lawrence Berkeley National Laboratory,University of California, Berkeley, CA 94720, USAe-mail: email@example.comR.J. Brodd (ed.), Batteries for Sustainability: Selected Entries from the Encyclopedia 5of Sustainability Science and Technology, DOI 10.1007/978-1-4614-5791-6_2,# Springer Science+Business Media New York 2013
6 M.M. DoeffIntercalation Originally, this referred speciﬁcally to layeredcompound structures that can undergo insertion of ions or(host material, molecules between the van der Waals gaps, but isinsertion compound) now commonly used for any structure that undergoes topotactic insertion reactions. For Li-ion battery materials, it refers speciﬁcally to compounds that undergo reductive insertion of lithium ions, such as graphite (used as an anode) or LiCoO2 (used as a cathode).Jahn–Teller effect The geometric distortion of nonlinear complexes of certain transition metal ions to remove degener- acy. For example, Mn(III) in octahedral coordina- tion is expected to have an electronic conﬁguration of t2g3eg1. Elongation along one axis of the octahe- dron, for example, decreases the symmetry and removes the degeneracy.Power density Power per unit volume or weight, respectively,and speciﬁc power often expressed as W/L or W/kg. Power is the product of the current and the operating voltage. This is a function both of the materials used and the cell design.Practical energy density Based on the entire weight or volume of the deviceor speciﬁc energy including inert components. It may be only 1/4–1/2 of the theoretical energy density. It may also refer only to the useable portion of the theoretical capac- ity of the anode or cathode material itself.Ragone plot A plot showing the relationship between energy density and power density for any particular bat- tery chemistry. This relationship is a function both of battery design and chemistry for Li-ion batteries.Solid electrolyte A very thin (nanometer scale) layer formed oninterface (SEI) a lithium or lithiated graphite anode, which develops upon reaction with certain kinds of electrolytic solutions. The SEI is a speciﬁc kind of reaction layer that is ionically conductive but electronically insulating. It passivates the electrode, preventing further reaction with the electrolytic solution, and allows reversible operation of the device.Speciﬁc capacity The amount of charge per unit weight that a battery electrode material contains, often expressed as mAh/g. This is a fundamental characteristic of the material, and depends upon its redox chemistry and structure.
2 Battery Cathodes 7Theoretical energy density, Based on weight or volume of the electrode activespeciﬁc energy, capacity materials only.Topotactic transformation A transformation in a crystal lattice involving displacement or exchange of atoms, which maintains the basic structure.Deﬁnition of the Subject and Its ImportanceIn a discharging battery, the cathode is the positive electrode, at which electro-chemical reduction takes place. As current ﬂows, electrons from the circuit andcations from the electrolytic solution in the device move toward the cathode.Although these processes are reversed during cell charge in secondary batteries,the positive electrode in these systems is still commonly, if somewhat inaccurately,referred to as the cathode, and the negative as the anode. Because this terminologyis widespread throughout the Li-ion battery literature, this usage will be adopted forthis article. Li-ion batteries are dual intercalation systems, in which both the cathode and theanode have structures that allow reversible insertion and extraction of lithium cations.In principle, there are numerous materials that undergo reversible intercalation andcan serve as electrode materials. Hence the chemistry of the Li-ion battery is not ﬁxed,unlike the great majority of battery systems. The choice of cathode greatly affects theperformance and cost of a Li-ion battery; for example, it is a major determinant ofenergy density, since it typically has a lower speciﬁc capacity than the most commonanode material, graphite (372 mAh/g), to which it must be matched.IntroductionThe very high theoretical capacity of lithium (3,829 mAh/g) provided a compellingrationale from the 1970s onward for the development of rechargeable batteriesemploying the elemental metal as an anode. The realization that some transitionmetal compounds undergo reductive lithium intercalation reactions reversiblyallowed the use of these materials as cathodes in these devices, most notably,TiS2 [1–3]. Another intercalation compound, LiCoO2, was described shortly there-after [4, 5] but, because it was produced in the discharged state, was not consideredto be of interest by battery companies at the time. Due to difﬁculties with the rechargeability of lithium and related safetyconcerns, however, alternative anodes were sought. The graphite intercalationcompound (GIC) LiC6 was considered an attractive candidate  but the highreactivity with commonly used electrolytic solutions containing organic solvents
8 M.M. Doeff 1000 6 4 IC Engine-2500 Wh / kg 100 h Fuel Cells EV goal 2 Specific Energy (Wh / kg) Li-ion PHEV-40 goal 100 6 PHEV-10 goal Ni-MH EV - Electric Vehicle 4 HEV - Hybrid-Electric Lead-Acid HEV goal Vehicle 2 10 h PHEV - Plug-in Hybrid- Electric Vehicle 10 Capacitors 6Range 4 1h 0.1 h 36 s 2 3.6 s 1 0 10 101 102 103 104 Specific Power (W / kg) Source: Product data sheets AccelerationFig. 2.1 A Ragone plot, showing the relationship between speciﬁc power and speciﬁc energy forseveral types of electrochemical devices. Goals set by FreedomCar for HEV, PHEVs, and EVs arealso indicated (Used with permission from )was recognized as a signiﬁcant impediment to its use. The development ofelectrolytes that allowed the formation of a solid electrolyte interface (SEI) onsurfaces of the carbon particles was a breakthrough that enabled commercializationof Li-ion batteries . In 1990, Sony announced the ﬁrst commercial batteriesbased on a dual Li-ion intercalation system . These devices are assembled in thedischarged state, so that it is convenient to employ a prelithiated cathode such asLiCoO2 with the commonly used graphite anode. After charging, the batteries areready to power devices. The practical realization of high energy density Li-ion batteries revolutionizedthe portable electronics industry, as evidenced by the widespread market penetra-tion of mobile phones, laptop computers, digital music players, and other light-weight devices, since the early 1990s. In 2009, worldwide sales of Li-ion batteriesfor these applications alone were US$7 billion . Furthermore, their performancecharacteristics (Fig. 2.1) make them attractive for traction applications such ashybrid electric vehicles (HEVs), plug-in hybrid electric vehicles (PHEVs), andelectric vehicles (EVs); a market predicted to be potentially ten times greater thanthat of consumer electronics. In fact, only Li-ion batteries can meet therequirements for PHEVs as set by the US Advanced Battery Consortium(USABC), although they still fall slightly short of EV goals. In the case of Li-ion batteries, the trade-off between power and energy shownin Fig. 2.1 is a function both of device design and the electrode materials that areused. Thus, a high-power battery (e.g., one intended for an HEV) will notnecessarily contain the same electrode materials as one designed for high energy(i.e., for an EV). As is shown in Fig. 2.1, power translates into acceleration, andenergy into range, or miles traveled, for vehicular uses. Furthermore, perfor-mance, cost, and abuse-tolerance requirements for traction batteries  differconsiderably from those for consumer electronics batteries. Vehicular
2 Battery Cathodes 9applications are particularly sensitive to cost; currently, Li-ion batteries are pricedat about US $1,000/kWh, whereas the USABC goal is US $150/kWh . Thethree most expensive components of a Li-ion battery, no matter what the conﬁgu-ration, are the cathode, the separator, and the electrolyte . Reduction of costhas been one of the primary driving forces for the investigation of new cathodematerials to replace expensive LiCoO2, particularly for vehicular applications.Another extremely important factor is safety under abuse conditions such asovercharge. This is particularly relevant for the large battery packs intended forvehicular uses, which are designed with multiple cells wired in series arrays.Premature failure of one cell in a string may cause others to go into overchargeduring the passage of current. These considerations have led to the developmentof several different types of cathode materials, as will be covered in the nextsection. Because there is not yet one ideal material that can meet requirements forall applications, research into cathodes for Li-ion batteries is, as of this writing,a very active ﬁeld.Characteristics of Battery Cathode MaterialsModern cathode materials for Li-ion batteries are generally prepared in the lithiated(discharged) state, so that they can be paired with delithiated anodes such as graphite.For ease of handling, it is desirable that the material be reasonably air-stable at roomtemperature. Furthermore, graphite anodes impose a penalty of approximately 0.1 V inaverage cell potential compared to Li metal. To compensate for this, and also tomaximize energy density, cathodes intended for use in Li-ion batteries have higheraverage potentials versus Li/Li+ than earlier materials such as TiS2 and vanadates developed for Li metal batteries. Furthermore, the requirement for high speciﬁc capac-ity generally restricts choices to compounds containing ﬁrst-row transition metals(usually Mn, Fe, Co, and Ni). Environmental and toxicity concerns have precludedthe development of most V or Cr-containing materials, although electroactivecompounds containing these metals exist. Today’s technologically important cathodesfall into two broad categories: metal oxides and polyanionic compounds. Figure 2.2 shows representations of the crystal structures of the most commonlyused cathode materials for Li-ion batteries, and Table 2.1 summarizes their generalproperties. Figure 2.3 shows typical discharge proﬁles of selected materials inLi half-cell conﬁgurations.Layered Transition Metal OxidesLiCoO2 was the ﬁrst of the layered transition metal oxides to be commercialized,and is still used today in batteries for consumer devices. It has the structure shownin Fig. 2.2a, where Co and Li, located in octahedral sites, occupy alternating layers
10 M.M. Doeff a b cFig. 2.2 Structures of common cathode materials: (a) The layered structure of LiCoO2 with c-axisoriented vertically. The octahedrally coordinated Li ions in 3a sites are represented as spheres andCoO6 (Co in 3b sites) as octahedra; (b) the cubic structure of LiMn2O4 spinel, with tetrahedrallycoordinated Li ions (in 8a sites) represented as spheres, and MnO6 (Mn in 16d sites) as octahedra;and (c) the olivine structure of LiFePO4, looking down the b-axis. Octahedrally coordinatedLi ions are represented as spheres, and FeO6 and PO4 as octahedra and tetrahedra, respectivelyTable 2.1 Characteristics of commercial Li-ion battery cathode materials Speciﬁc Potential versus capacity, SpeciﬁcMaterial Structure Li/Li+, average V mAh/g energy, Wh/kgLiCoO2 Layered 3.9 140 546LiNi0.8Co0.15Al0.05O2 (NCA) Layered 3.8 180–200 680–760LiNi1/3Co1/3Mn1/3O2 (NMC) Layered 3.8 160–170 610–650LiMn2O4 and variants (LMO) Spinel 4.1 100–120 410–492LiFePO4 (LFP) Olivine 3.45 150–170 518–587 4.5 4 3.5 Cell Potential, V 3 2.5 LiFePO4 Li1+xMn2–xO4 2 LiNi1/3Co1/3Mn1/3O2 1.5 0 20 40 60 80 100 120 140 160 Specific Capacity, mAh/gFig. 2.3 Discharge proﬁles of lithium cells containing LiFePO4, Li1+xMn2ÀxO4, or LiNi1/3Co1/3Mn1/3O2 electrodes
2 Battery Cathodes 11along the 111 planes in a cubic close-packed (ccp) oxygen array, to form a structurewith overall hexagonal symmetry (space group R-3m). This type of stackingarrangement is called O3 in layer notation, indicating that there are three transitionmetal layers per unit cell and the Li ions are octahedrally coordinated. Delithiation proceeds topotactically [15, 16] and is reversible over the composi-tion range 1 ! x ! $0.5 for x in LixCoO2, giving a practical speciﬁc capacity ofabout 140 mAh/g below 4.2 V versus Li/Li+. Extraction of lithium to values of x <$0.5 results in higher practical capacities initially, but often increases cyclinglosses . This has been attributed to side reactions involving particle surfaces,which increase cell impedance, and to structural instability associated with phasechanges at very low values of x in LixCoO2 [18–21]. Coating LiCoO2 particles, orrigorous heat treatment to remove surface species [22–24], results in improvedcycling below 4.5 V versus Li/Li+, but full delithiation is still not possible withoutcycling losses. A layered compound with the nominal composition of LiNiO2 has also beenextensively studied for battery applications [25–28]. Its lower cost compared toLiCoO2, and the potential for higher energy density were driving forces for itsdevelopment. Although the structure is similar to LiCoO2, LiNiO2 readily exhibitsnon-stoichiometry. During synthesis, there is a tendency toward loss of lithium andreduction of some Ni to the +2 oxidation state. The Ni2+ migrates to Li+ 3a sites, dueto the similarities in size between the two types of ions. The actual composition canbe written as Li1ÀzNi1+zO2 with 0 < z < 0.2, or as (Li1ÀzNiz2+)3a(Niz2+Ni1Àz3+)3bO2. The degree of disorder is inﬂuenced by the synthetic conditions, and theelectrochemical properties (e.g., the ﬁrst cycle reversibility) are affected by thedegree of non-stoichiometry [30, 31]. The difﬁculty in synthesizing high-qualityLiNiO2 was one impediment to its widespread adoption as a cathode material inLi-ion batteries, although nearly ideal structures can be obtained if sufﬁcient care istaken . (However, perfectly stoichiometric LiNiO2 materials probably do notexist). Partial substitution of Ni with Co  was later found to be effective atreducing the cationic disorder on 3a sites, leading to compositions such asLiNi0.8Co0.2O2. Cobalt also helps to reduce oxygen loss at high states-of-charge,improving safety. The thermal instability of LixNiO2 at high states-of-charge [33–36] also raiseda great deal of concern about the safety of this material when used as a cathode. Theproperties of LiNiO2 have been improved via coating and doping with Mg, leadingto a very high-capacity electrode material  with better thermal properties.However, the most commonly used electrode material related to LiNiO2 isLiNi0.8Co0.15Al0.05O2 or NCA, which is now commercially produced (see Table 2.1for general properties). The presence of Al in NCA improves both the thermal[33–36] and electrochemical properties [38, 39]. The high speciﬁc capacity andgood power capability of this material make it attractive for vehicular applicationsalthough it is still not considered as inherently safe as other candidates such as LFP(see Table 2.2 and the discussion of olivines below). Several ternary Li-Fe-O phases exist with differing arrangements of cations incubic close-packed oxygen arrays . However, LiFeO2 with the R-3m structure
12 M.M. DoeffTable 2.2 Relative merits of selected commercial Li-ion battery cathodesAdvantages DisadvantagesLMO (LiMn2O4 and variants)Low cost Mn solubility issue, affecting cycle lifeExcellent high rate performance Low capacityHigh operating voltageNo resource limitationsModerate safety (oxygen release)LFP (LiFePO4 and variants)Moderately low cost Low operating voltageExcellent high rate performance Low capacity, especially for substituted variantsNo resource limitations Controlling patentsVery slow reaction with electrolyteExcellent safety (no oxygen release)NMC (LiNi1/3Co1/3Mn1/3O2) and variantsHigh capacity High cost of Ni and CoHigh operating voltage Potential resource limitationsSlow reaction with electrolytes Relatively new in performanceModerate safety (oxygen release) Controlling patentsNCA (LiNi0.8Co0.15Al0.05O2)Performance is well established High cost of Ni and CoSlow reaction with electrolytes Potential resource limitationsHigh capacity Controlling saft patentsHigh voltageExcellent high rate performanceis metastable and generally must be prepared via indirect methods such as ionexchange of NaFeO2. The electrochemical properties of this material  and mostother polymorphs [42, 43] are not, however, suitable for lithium-ion batteries due tolow and highly sloping voltage proﬁles or poor cycling properties. Li5FeO4 with theanti-ﬂuorite structure has a potential proﬁle that may be compatible in a Li-ionbattery conﬁguration, but delithiation does not appear to proceed via simple oxida-tive deintercalation . This material has been proposed for use as a lithium-ionsource for lithium-ion batteries (i.e., to lithiate graphite anodes so that cathodes inthe charged state may be used). Ternary Li-Mn-O phases with Mn in the +3 or +4 oxidation state crystallize asspinels, the rock salt structure Li2MnO3, or as orthorhombic LiMnO2 witha corrugated structure (o-LiMnO2) but not as O3 layered structures. Lithiummanganese oxide spinels (LMO) are technologically important cathodes and willbe considered in a later section (vide infra). The Na-Mn-O system contains numer-ous polymorphs, including layered structures. NaMnO2 has the same stackingarrangement as LiCoO2, but is monoclinically distorted (space group C2/m), dueto the abundance of Jahn–Teller distorted Mn3+ ions. Ion exchange of this com-pound yields a layered LiMnO2 (designated O’3, with the prime indicating themonoclinic distortion) , but it rapidly converts to spinel upon electrochemicalcycling, as does orthorhombic LiMnO2 . O’3-LiMnO2, o-LiMnO2, and spinelmanganese oxide all have cubic close-packed oxygen arrays and differ only in the
2 Battery Cathodes 13cation arrangement. Upon electrochemical delithiation of the ﬁrst two materials,disproportion of Mn3+ into Mn2+ and Mn4+ ions occurs and Mn2+ ions subsequentlymigrate into vacant sites in the lithium layers via low-energy pathways, facilitatingstructural rearrangement to spinel . Lithium-deﬁcient layered LixMnO2+y (x%0.7, y ! 0.05), which has an O2 ratherthan O3 stacking arrangement, does not convert to spinel upon cycling [48, 49],because the oxygen array is not ccp. In addition, non-stoichiometric lithium man-ganese oxides that are intergrowths of O2 and O3 phases show better resistance toconversion than the pure O3 structure [50, 51]. The presence of transition metalvacancies in these compounds (which reduce the concentration of the Jahn–TellerMn3+ ions) results in low rate capability, because the vacancies tend to trap nearbylithium ions, impeding their mobility . Other lithium manganese oxides with tunnel structures [53–55] exhibit interest-ing electrochemical properties, particularly those based on the Na0.44MnO2 struc-ture. This material has excellent cycling characteristics  and rate capability, and does not convert to spinel, although the practical capacity is limited byvoltage considerations (the average potential at which lithium is extracted is thehighest of any known manganese oxide ). All of these tunnel and O2 or O2/O3layered materials, however, must be prepared via ion exchange of their sodiummanganese oxide structural analogs, complicating their preparation. Furthermore,the lithium deﬁciency of the ion-exchanged materials limits the capacity in Li-ionbattery conﬁgurations, as all of the cycleable lithium must originate fromthe cathode. Li2MnO3 can be considered a layered structure similar to LiCoO2, but with 111planes alternately occupied by Li and Li1/3Mn2/3. Ordering of Li and Mn in thetransition metal layer imposes a monoclinic superstructure, but the stackingarrangement is essentially identical to that of the R-3m structures discussedabove. Mn in this compound is tetravalent and all lithium sites are occupied,precluding either oxidative deintercalation or reductive intercalation. Nevertheless,several researchers have observed electrochemical activity of Li2MnO3 when it ischarged in lithium half-cells to high potentials . Recent evidence  suggeststhat lithium deintercalation occurs with simultaneous oxygen loss during the initialcharge, as well as H+/Li+ exchange. The converted material becomes electroactiveand can subsequently be lithiated during cell discharge. Acid leaching of Li2MnO3also yields an electroactive manganese oxide phase . The reaction involvesloss of Li2O from the structure and ion exchange, to produce layeredH1ÀxLix[Li0.33Mn0.67]O2 . The compound Li1.2Mn0.4Cr0.4O2  is essentially a solid solution of layeredLi2MnO3 and LiCrO2 with an O3 stacking arrangement . Very high dischargecapacities ($200 mAh/g) can be obtained based on Cr3+$Cr6+ redox processes.Conversion to spinel phases does not occur because Mn remains in the +4 oxidationstate throughout charge and discharge, nor does the electrode need chemical orelectrochemical activation prior to use. Nevertheless, concerns over the environ-mental impact of hexavalent chromium have prevented further development of thismaterial.
14 M.M. DoeffFig. 2.4 A transition metal layer in LiNi0.5Mn0.5O2 showing the ﬂower pattern. Li is representedby the large gray circles, Mn by small white circles, and Ni by black circles (Used with permissionfrom Ref. ) The search for improved layered oxide materials containing low-cost transitionmetals ultimately led to the discovery of LiNi0.5Mn0.5O2 [65–67] as wellas compounds with the general composition Li[NixLi(1/3À2x/3)Mn(2/3Àx/3)]O2 .Computational modeling  and spectroscopic investigations  show that theNi and Mn in these materials are in the +2 and +4 oxidation states, respectively.During normal charge processes in an electrochemical cell, nickel is ultimatelyoxidized to the +4 oxidation state, and Mn remains tetravalent. LiNi0.5Mn0.5O2 doesnot convert to spinel upon cycling, unlike the metastable O3-LiMnO2, because notrivalent Mn is ever produced in the structure. The defect chemistry of LiNi0.5Mn0.5O2 also distinguishes it from LiNiO2(where nickel is primarily in the +3 oxidation state initially) discussed above.A feature of LiNi0.5Mn0.5O2 is anti-site mixing [65–67, 71, 72] in which someNi2+ ions are located on the Li 3a sites, and some Li+ ions on transition metal 3bsites, that is, (Li1ÀxNix)3a(LixNi0.5ÀxMn0.5)3bO2, x%0.08À0.12. Mn ions in thetransition metal layers preferentially surround the Li ions located in 3a sites toform Li2MnO3-like clusters, and Ni ions occupy sites adjacent to Mn, to forma “ﬂower pattern” (Fig. 2.4). The anti-site mixing is thought to be a thermodynami-cally favored feature of the ion ordering and thus intrinsic to the structure. Unlikewith LiNiO2, simple manipulation of conditions during direct synthesis is thereforenot likely to result in a near-ideal layered structure. Li[NixLi(1/3À2x/3)Mn(2/3Àx/3)]O2 compounds can be considered solid solutions ofLi2MnO3 and LiNi0.5Mn0.5O2. Although the discharge capacity between 4.4 and3.0 V versus Li/Li+ drops as the Ni content decreases, the opposite trend is observedafter cell charge to 4.8 V and subsequent discharge to 2.0 V . In addition, theLi2MnO3-rich materials exhibit a plateau at about 4.5 V during charge, the length ofwhich is inversely proportional to x. This is thought to be deintercalation of Li ionswith concomitant loss of oxygen (for a net loss of Li2O), similar to what happenswhen Li2MnO3 is charged in an electrochemical cell. This process can result in veryhigh discharge capacities upon subsequent cycles (e.g., 230 mAh/g for x = 1/3).
2 Battery Cathodes 15An advantage to these materials and related Li-rich materials (where excess lithiumreplaces some of the transition metal ions on 3b sites, but the Mn content still equalsthat of the Ni content) is decreased cation mixing. This improves rate capability as compared to LiNi0.5Mn0.5O2. The presence of a relatively large number of Ni ions in the Li 3a sites of theLiNi0.5Mn0.5O2 structure due to the anti-site mixing has a negative impact on theLi diffusivity, resulting in a low-rate cathode material. LiNi0.5Mn0.5O2, prepared bylow-temperature ion exchange of the nearly perfectly layered NaNi0.5Mn0.5O2analog, is capable of sustaining higher discharge currents than samples preparedby conventional methods . However, the most successful method used toaddress this issue has been to incorporate some cobalt into the structure . Thebest known of these compounds is Li[Ni1/3Co1/3Mn1/3]O2, sometimes referred to asNMC (Tables 2.1 and 2.2). This compound is gradually replacing LiCoO2 inconsumer batteries (in some cases, a mixture of the two are used as the cathode)and is under consideration for some vehicular applications. The voltage proﬁle ofNMC versus Li/Li+ is gradually sloping (Fig. 2.3), as is typical of many layeredcompounds, and provides a somewhat higher capacity than LiCoO2 below 4.3 Vversus Li/Li+ (typically about 160 mAh/g compared to 140). Capacities in excess of200 mAh/g can be achieved when cells are charged to higher voltage limits,although this usually results in diminished cycle life. The oxidation states of Ni, Co, and Mn in as-made Li[Ni1/3Co1/3Mn1/3]O2 are+2, +3, and +4, respectively . First principle calculations suggest that Ni2+ isultimately oxidized to Ni4+ during extraction of the ﬁrst two-thirds of the lithiumduring electrochemical charging in lithium cells, and oxidation of Co3+ to Co4+occurs only during removal of the last one-third  (i.e., at high cell potentials).As in LiNi0.5Mn0.5O2, Mn remains inactive throughout normal operating cellvoltages. The redox activity of Ni during the extraction of lithium from Li[Ni1/3Co1/3Mn1/3]O2 has been veriﬁed by in situ X-ray absorption spectroscopic (XAS)studies, although the details of the participation of Co in the electrochemistry areless clear [79–83]. Charge compensation associated with Co is currently thought tooccur, at least partially, at oxygen sites, due to the covalency of the Co-O bonds. The improved electrochemical properties and better structural, chemical, andthermal stability [84, 85] of Li[Ni1/3Co1/3Mn1/3]O2 compared to LiCoO2 or NCArender it an attractive replacement cathode material for consumer batteries. Never-theless, the presence of a signiﬁcant amount of costly cobalt, albeit in reducedquantities compared to LiCoO2, may still make it too expensive for most vehicularapplications. Compounds having the general formula Li[NixCo1À2xMnx]O2 withx ¼ 0.4 or 0.45 have recently been developed by Whittingham and coworkersspeciﬁcally to address the cost issue [86–89]. Although the amount of anti-sitemixing increases with larger x, these materials exhibit very good electrochemicalperformances. The effect of increasing the Ni content of these materials on thethermal stability, especially at high states of charge, remains to be determined,however. Another approach has been to partially substitute another metal such asaluminum for cobalt [89, 90]. Although the amount of substitution must be kept
16 M.M. Doefflow to maintain the high speciﬁc capacities, both the thermal stability of thedelithiated materials  and the electrochemical properties [92, 93] appear to beenhanced. All of the NMCs discussed above contain equal amounts of Ni and Mn, whichensure that the oxidation states of the two metals are primarily +2 and +4, respec-tively. Recent attempts to increase Mn content in stoichiometric materials havingthe formula Li[Ni0.45ÀxCo0.1Mn0.45+x]O2 yielded phase mixtures for values of x >0.05  and a solid solution phase for x = 0.05. In this compound, Li[Ni0.4Co0.1Mn0.5]O2, the extra manganese is in the +3 oxidation state. Unfortu-nately, this material exhibits poorer capacity retention upon electrochemicalcycling and lower rate capability than Li[Ni0.45Co0.1Mn0.45]O2. It is,however, possible to form solid solutions between Li[Ni1/3Co1/3Mn1/3]O2 andLi2MnO3 to make Li- and Mn-rich materials where the excess Mn is in the +4oxidation state. As with the related Li[NixLi(1/3À2x/3) Mn(2/3Àx/3)]O2 compounds,these materials can be electrochemically activated during charge to high potentialsin lithium cells. The activation process (deintercalation of Li, concomitant loss ofoxygen, and H+/Li+ ion exchange) yields electrodes with discharge capacities ashigh as 290 mAh/g [95, 96]. The very high capacities make these materialsinteresting for both consumer and automotive applications, and they are nowbeing actively developed (e.g., by Envia Systems, Newark, CA).Manganese Oxide SpinelsThe marked tendency for many manganese oxide phases to convert to spinelstructures during lithiation in electrochemical cells, or upon heating witha lithium source, attests to the stability of this structure in the Li-Mn-O system.The stoichiometric spinel, LiMn2O4, is easily synthesized in air from a variety of Liand Mn-containing precursors. Figure 2.2b shows its cubic structure (space groupFd-3m), where Li ions occupy tetrahedral 8a sites and Mn is located in octahedral16d sites in a ccp array of oxygen anions. In addition, there are vacant tetrahedraland octahedral interstitial sites in the three-dimensional structure that providepathways for lithium diffusion. Early work  showed that it is possible to remove lithium from LiMn2O4using a mild acid treatment. During this process, Mn is oxidized from an average+3.5 oxidation state to +4, and l-MnO2, which retains the spinel framework, isformed (Eq. 2.1). In addition, some dissolution of Mn occurs: 2LiMn2 O4 þ 4Hþ ðaqÞ ! 2Liþ ðaqÞ þ Mn2þ ðaqÞ þ 2H2 O þ 3 l-MnO2 (2.1) Oxidative extraction of lithium from the tetrahedral 8a sites of LiMn2O4 to forml-MnO2 in a lithium cell [98, 99] was subsequently demonstrated to occur slightlyabove 4 V. It is also possible to insert lithium into the vacant octahedral sites of
2 Battery Cathodes 17Fig. 2.5 Discharge proﬁle of 4.5a Li/modiﬁed-LiMn2O4 cellat 0.1 mA/cm2. Cell was 4initially discharged to 2 V and Cell Potential, Vthen charged to 4.3 V. Thiswas the third discharge 3.5between 4.3 and 2.0 V 3 2.5 2 0 50 100 150 200 Specific Capacity, mAh/gLiMn2O4 either chemically or electrochemically, with concomitant reduction ofMn. When carried out in a cell with a lithium anode, this process occurs below 3 V,and the discharge proﬁle is ﬂat, indicative of a two-phase reaction. The tetragonallydistorted phase Li2Mn2O4 (space group I41/amd) is formed due to the cooperativeJahn–Teller effect, which occurs when more than half the manganese is in the formof d4 Jahn–Teller Mn3+ ions. The phase transition results in a 16% increase in the ˚ ˚ ˚c/a ratio  (a = c = 8.248 A in LiMn2O4; a = 8.007 A, c = 9.274 A in Li2Mn2O4).In theory, lithium cells containing LiMn2O4 can either be charged or dischargedinitially, and then cycled over a composition range of 0 x 2 in LixMn2O4 to givea total speciﬁc capacity of 285 mAh/g. Figure 2.5 shows the voltage proﬁle ofa Li/modiﬁed LiMn2O4 cell assembled in the author’s laboratory, after discharginginto the 3 V region and full recharge. Both 4 and 3 V plateaus are evident; althoughthe overall capacity is somewhat lower than the theoretical value. The large anisotropic volume change associated with formation of tetragonalLi2Mn2O4 results in particle disintegration and loss of connection within thecomposite electrode. This causes such a rapid loss of capacity that, in practice,the cycle lives of cells containing LiMn2O4 discharged even a few times into the3 V region are greatly compromised. In contrast, the extraction of lithium fromLiMn2O4 above 4 V versus Li/Li+ maintains the cubic structure and results insmaller volume changes. For this reason, discharge is typically limited to the 4 Vplateau (Fig. 2.3), which exhibits much better reversibility. The theoretical capacityassociated with this plateau is 148 mAh/g, although it is difﬁcult to fully extract allthe lithium, resulting in somewhat lower practical values. From the early 1990s onward, intensive efforts were devoted to the developmentof LiMn2O4 for lithium-ion batteries, particularly at Bellcore Laboratories[101–103]. Although limiting discharges to the 4 V plateau resulted in much bettercycling than when both the 3 and 4 V plateaus were utilized, gradual capacityfading was still observed . This behavior was attributed to several factors,including irreversible side reactions with the electrolyte due to the high potential,loss of oxygen from the delithiated spinel, dissolution of Mn, and production
18 M.M. Doeff 1.15 3.60Li content, 1+x, in Li1–xMn2–xO4 Manganese Oxidation State 1.10 3.58 1.05 3.56 1.00 3.54 0.95 3.52 0.90 3.50 8.2 8.21 8.22 8.23 8.24 8.25 8.2 8.21 8.22 8.23 8.24 8.25a Lattice Parameter, Å b Lattice Parameter, Å 50 40 % Capacity Loss 30 20 10 0 8.2 8.21 8.22 8.23 8.24 8.25 c Lattice Parameter, ÅFig. 2.6 (a) The variation of the lattice parameter, a, with the lithium content of Li1+xMn2ÀxO4;(b) the variation of lattice parameter with the average Mn oxidation state in Li1+xMn2ÀxO4; and(c) relationship between capacity loss after 120 cycles and the lattice parameter in Li1+xMn2ÀxO4(Used with permission from Ref. )of tetragonal Li2Mn2O4 at particle surfaces, particularly at high discharge rates[100, 105]. Partial substitution of Mn to form LiMxMn2ÀxO4 improves capacity retention[106–112]. Of particular interest are the lithium-substituted materials having thegeneral formula Li1+xMn2ÀxO4. As lithium is substituted for manganese on the 16dsites (x is increased), the average oxidation state of the latter rises. This effectivelydecreases the 4 V capacity in proportion to the amount of substitution but results ina higher average oxidation state of the Mn at the end-of-discharge. This amelioratesthe tendency to form the tetragonally distorted phase under nonequilibriumconditions such as rapid discharging, because this occurs only when the Mnoxidation state falls below an average of 3.5. Because Mn is fully oxidized beforeall the lithium can be extracted from 8a sites, side reactions are suppressed. Finally,dissolution of Mn decreases because this phenomenon is dependent on the concen-tration of trivalent ions. Li substitution and the attendant increase in Mn oxidation state in the as-madeLi1+xMn2ÀxO4 compounds decrease the lattice parameter, a (Fig. 2.6a and b). Themagnitude of this value correlates closely with the amount of capacity loss uponcycling (Fig. 2.6c), so that it can be used to predict the cycling behavior of thespinel materials . In particular, improvements are most marked when a 8.23 A. ˚Because the cycling behavior is so much better than LiMn2O4, nearly all commercial
2 Battery Cathodes 19manganese oxide spinel materials (LMOs) made today are lithium substituted. Thesehave theoretical speciﬁc capacities of 100–120 mAh/g (Table 2.1), somewhat lowerthan that for LiMn2O4. The maximum possible substitution in Li1+xMn2ÀxO4 corresponds to x = 1/3(the compound Li4/3Mn5/3O4 or Li4Mn5O12), at which point all of the Mn is in the+4 oxidation state and there is no 4 V capacity, because oxidative extraction oflithium cannot occur. Nevertheless, it is possible to insert lithium reversibly intooctahedral 16c sites at about 2.9 V versus Li/Li+ until a composition of Li7Mn5O12is reached, for a total of 156 mAh/g [114, 115]. The cubic symmetry is maintaineduntil about Li6.5Mn5O12, at which point Mn is reduced to an average oxidation stateof 3.5 and the cooperative Jahn–Teller effect induces a tetragonal distortion.Because this process occurs only at the end-of-discharge, Li4Mn5O12 exhibitsmuch better cycling behavior on the 3 V plateau than does LiMn2O4. However,the low operating voltage and capacity, and the inability to extract lithium makesLi4Mn5O12 impractical for Li-ion batteries. It is also possible to prepare cation-deﬁcient or defect spinels, Li1ÀxMn2À2xO4. The cation vacancies increase the average oxidation state of Mn and decreasethe capacity above 4 V in favor of that below 3 V, proportionally with x. In the end-member compound Li2Mn4O9 (corresponding to x = 0.11 in Li1ÀxMn2À2xO4), allMn is tetravalent, and lithium cannot be extracted, so that there is no capacity at4 V. Lithium can be inserted below 3 V versus Li/Li+, to a maximum compositionof Li5Mn4O9. Although the theoretical capacity (213 mAh/g) is higher than that ofLi4Mn5O12, approximately 1/3 of it is associated with the formation of theJahn–Teller distorted tetragonal phase. In principle, defect spinels with values of x < 0.11 should cycle on the 4 Vplateau better than LiMn2O4 for the same reasons as the lithium-rich stoichiomet-ric spinels. In practice, it is difﬁcult to control the degree of non-stoichiometryduring synthesis, so these materials are not of interest commercially. In spite of the improved performance exhibited by the lithium-substitutedspinels, capacity fading upon cycling is still observed in electrochemical cells,particularly at elevated temperatures (55 C) [116–121]. This has negativeimplications particularly for vehicular applications, where batteries may besubjected to a wide variety of operating and storage conditions, including verywarm environments. The dissolution is associated with Mn3+ disproportionation(Eq. 2) in the presence of acidic components of the LiPF6/organic carbonateelectrolyte solutions used in Li-ion batteries. 2Mn3þ ðsolidÞ ! Mn4þ ðsolidÞ þ Mn2þ ðsolutionÞ (2.2) Loss of manganese leads to the formation of a defect spinel structure withreduced or no 4 V capacity [104, 116–121]. Additionally, proton exchange[116–121], phase separation, ﬁlm formation, and precipitation of MnO and MnF2may occur, increasing cell impedance and exacerbating the capacity fading. Moresigniﬁcantly, dissolved Mn2+ can cross over to the anode, become reduced, and
20 M.M. Doeffprecipitate as the metal, increasing the charge-transfer resistance and disrupting thecritical SEI layer [122, 123]. The graphite anode is markedly more sensitive to thiseffect than lithium is. Thus, assessment of spinel cathodes to determine the effec-tiveness of an approach to improve resistance to dissolution should ultimately becarried out in a full cell conﬁguration rather than in lithium half-cells. Some methods designed to address the problem of spinel dissolution includecoating of particles [124, 125] and the use of new non-ﬂuorinated salts such aslithium bis(oxalato)borate (LiBOB) which do not generate HF in situ [126–128].Interestingly, dissolution of manganese appears to be suppressed in electrodeswhere LMO is mixed with an NMC . Although the cycling behavior of Li-ion cells with spinel electrodes is still inferior to that of devices containingalternative commercial cathode materials (Table 2.2), other aspects of performancesuch as rate capability and safety [33–36, 130], the wide availability of manganeseprecursors, and the potential for low cost make LMO attractive especially forvehicular applications. Thus, at least one battery manufacturer focused on vehicletechnologies (e.g., Enerdel, Indianapolis, IN) is pursuing the development of Li-ionbatteries with spinel cathodes and hard carbon anodes (which are less sensitive tothe effects of manganese dissolution than graphite). Several lithium-containing oxide spinels having transition metals other than Mncan also be synthesized. One example is LiCo2O4, which can be prepared froma low-temperature form of LiCoO2 . (The latter, known as LT-LiCoO2, hasa structure intermediate between that of a spinel and layered compound). Another isLiNi2O4 . Unlike LiMn2O4, the electrochemical characteristics of most of thesespinels are inferior to those of the layered analogs, so that they are not of techno-logical interest as cathode materials. However, Li4Ti5O12 (LTO), which, because ofits voltage properties, functions as an anode material, demonstrates excellentcycling performance. Although the energy density is lower than that of graphite,it does not require the formation of an SEI. Thus, it is also an attractive match forLMO cathode materials. Batteries with LTO anodes and LMO or other high-voltagecathodes may ﬁnd utility in HEVs, which do not require as high an energy densityas pure EVs. The intensive search for substituted lithium manganese spinels with bettercycling performance led to the discovery of several materials having capacitynear 5 V versus Li/Li+. These include spinels substituted with Cr, Fe, Cu, Co, orNi [132–136]. In most cases, these materials exhibit a plateau near 4 V as well asa second plateau near 5 V, with the magnitude of the latter increasing with larger xin LiMxMn2ÀxO4 (where M = Cr, Fe, Cu, Co, or Ni). The 4 V capacity is associatedwith the usual Mn3+/Mn4+ spinel redox couple, whereas the higher voltage plateauis associated with redox processes of the substituting metal. Interestingly, thecompound LiNi1/2Mn3/2O4 has very little 4 V capacity, unlike other LiM1/2Mn3/2O4spinels  (Fig. 2.7). In the case of LiNi1/2Mn3/2O4, nearly all of the Mn is tetravalent , so thatfurther oxidation is not possible. The speciﬁc capacity of 147 mAh/g at 4.7 V isassociated with Ni2+/Ni4+ redox processes. The high energy density and high voltagemakes this material attractive for vehicular applications, because fewer cells need to
2 Battery Cathodes 21a b c 1.0 1.0 1.0 0.5 0.5 0.5 4.05V I/mA I/mAI/mA 4.00V 4.92V 4.12V 5.00V 0.0 0.0 3.98V 0.0 −0.5 −0.5 −0.5 −1.0 −1.0 −1.0 3 4 5 3 4 5 3 4 5 E/V E/V E/Vd e f 1.0 1.0 1.0 0.5 0.5 0.5 3.96V 5.15V 4.80VI/mA I/mA I/mA 4.17V 0.0 0.0 3.95V ?? 0.0 3.92V 4.86V −0.5 −0.5 −0.5 −1.0 −1.0 −1.0 3 4 5 3 4 5 3 4 5 E/V E/V E/VFig. 2.7 Slow-scan voltammetry of Li/LiM1/2Mn3/2O4 cells with M = (a) Cr, (b) Mn, (c) Fe, (d)Co, (e) Ni, and (f) Cu at a rate of 0.2 mV/s using 1 M LiPF6 in 1:1 v/v EC/DEC electrolyte (Usedwith permission from Ref. )be connected in series to make the 300 V packs used in electric vehicles. Thissimpliﬁes engineering, results in comparatively higher energy density on the systemlevel because less hardware is required, and lowers costs. ETV Motors of Herzliya,Israel, is one company actively developing LiNi1/2Mn3/2O4 batteries for this purpose. The very high potential at which this cathode operates, however, presentsconsiderable challenges for cycle life. Although conventional carbonate-basedelectrolytes used in Li-ion batteries have, in principle, excellent oxidative stability,the presence of impurities such as water may contribute to side reactions thatdecrease resistance to irreversible oxidation, resulting in shortened batterylifetimes. In addition, cell components such as carbon additives used to improveconductivity in composite cathodes, or surfactants that aid in wetting may oxidizeirreversibly at high potentials, and current collectors may corrode. Thus, cycling isusually restricted to a voltage range below about 4.3 V versus Li/Li+ (4.2 V in cellswith graphite anodes). Stringent puriﬁcation of electrolytes and the use of specialprotective additives are allowing gradual extension of this range. In addition, thedevelopment of new electrolytes containing ionic liquids or sulfolanes is expectedto enable high-voltage cell operation, although the choice of anode may then be
22 M.M. Doeffrestricted to LTO or other materials that do not require SEI formation. Otherstrategies to prolong the cycle life of cells containing LiNi1/2Mn3/2O4 includetreating active material particles with protective coatings to minimize direct contactwith electrolyte solutions [138–140], or partial substitution of Ni or Mn with othercations such as Ti, Mg, or Zn [141–143]. Synthesis of LiNi1/2Mn3/2O4 is normally carried out at high temperatures toensure good crystallinity and to lower the surface area and thus minimize reactivitywith electrolyte solutions and other components. Under these conditions, oxygenloss may occur, leading to the formation of a non-stoichiometric material(LiNi1/2Mn3/2O4Àx) containing some Mn3+ in the structure. Additionally, a rocksalt impurity, LixNi1ÀxO, is also produced. Annealing at 700 C partially reversesthe oxygen loss, but the telltale 4 V capacity indicative of the presence ofelectroactive Mn3+ can often be observed in cells made with these materials (e.g.,in Fig. 2.7e). Substitution with other metals, as discussed in the papers listed inRefs. [141–143], often decreases the amount of Mn3+ in these compounds, whichmay play a role in the observed improvements in cycling. If the sample is cooled slowly during synthesis, an ordered phase can beproduced (space group P4332 with Ni in 4b sites and Mn in 12d sites ). Theelectrochemical properties (in particular, rate capability) of the ordered phase areinferior to those of the disordered non-stoichiometric phase [145, 146]. The mixedMn valency in the disordered Fd-3m phase leads to an increase in the electronicconductivity of about 1.5 orders of magnitude compared to that of the orderedmaterial. This is thought to be responsible for the increased rate capability of theformer compared to the latter. The presence of electroactive Mn in disordered LiNi1/2Mn3/2O4 suggests thatdissolution may be problematic, as it is with the LiMn2O4 variants. In spite of thisand the high operating voltages, extremely stable cycling has been observed in fullcell conﬁgurations, albeit with Li4Ti5O12 anodes .LiFePO4 and Other Phospho-olivinesIn 1997, Goodenough and coworkers reported on the electrochemical properties ofa new class of cathode materials known as the phospho-olivines , which adoptthe orthorhombic structure (space group Pnma) shown in Fig. 2.2c. In the case ofLiFePO4 (triphylite), Li+ and Fe2+ occupy octahedral sites, and P is located intetrahedral sites in a somewhat distorted hexagonal close-packed (hcp) oxygenarray. The FeO6 octahedra share corners and LiO6 octahedra share edges alongtunnels down the b-axis, through which the Li ions can diffuse. Extraction andreinsertion of Li from LiFePO4 proceeds at about 3.45 V in a lithium cell witha theoretical speciﬁc capacity of 170 mAh/g. The potential is independent of thecomposition x in LixFePO4 (i.e., the voltage proﬁle is ﬂat, Fig. 2.3) indicating thata two-phase reaction occurs. In situ X-ray diffraction and Mossbauer experiments
2 Battery Cathodes 23Fig. 2.8 Photographs ofLiFePO4 samples containingvarying amounts of carbon(Used with permission fromRef. )on Li/LiFePO4 cells  show that the two relevant phases are triphylite andFePO4, also known as heterosite (Eq. 2.3). LiFePO4 ðtriphyliteÞ $ FePO4 ðheterositeÞ þ eÀ þ Liþ (2.3) Initial reports on the electrochemical characteristics of LiFePO4 emphasized itspoor rate capability and the lower than expected utilization in lithium cells evenwhen discharged at low current densities (e.g., only about 60% in Ref. ). Thiswas attributed to the low electronic conductivities of both the triphylite andheterosite phases . Coating particles with carbon ameliorates the low conduc-tivity and result in better rate performance . This is most convenientlyachieved by including a carbon source during initial synthesis of the LiFePO4sample. The presence of carbon or carbon-containing precursors during calcinationin an inert atmosphere has several additional beneﬁcial effects; it retards graingrowth, resulting in small particles that allow rapid extraction of Li ions, andprevents formation of Fe3+-containing impurities. It also allows the use of easy-to-handle, low-cost, Fe3+-containing starting materials such as iron nitrate, whichare reduced during the heating process . In practice, many lab-synthesized samples of LiFePO4 contain carbon, due to theuse of precursors such as iron oxalate . Even small amounts of carbon canresult in drastic sample color changes from the off-white of native LiFePO4(Fig. 2.8). The electrochemical performance is also greatly affected by the carboncontent, although this also depends on the distribution of carbon over particlesurfaces and details of its structure [154–157]. Carbons produced in situ duringsynthesis of LiFePO4 are disordered due to the relatively low calcinationtemperatures (generally, 600–700 C). Disordered carbons are less conductivethan graphite, and conductivity depends on the size and number of graphenedomains. The use of graphitization catalysts (often containing iron) improves theconductivity of coatings by several orders of magnitude, and can also result in co-production of carbon nanotubes or ﬁbers, which wire particles together [158, 159].The result is that very small amounts of carbon, often less than 2 wt.%, are sufﬁcientto produce high-rate LiFePO4 samples. This is important because too much light-weight carbon adversely affects the tap densities of LiFePO4 composites, furtherdecreasing the already somewhat low energy density . The changes in sample color, increases in bulk conductivities, and improvedelectrochemical performance induced by the presence of very small amounts of
24 M.M. Doeffcarbon (or other highly colored impurities) complicate the interpretation of resultsof doping experiments intended to increase the intrinsic conductivity of LiFePO4.A color change from off-white to black or gray should not be regarded as proof-positive of successful doping and increased intrinsic electronic conductivity, for thereasons described above. Even when carbonaceous precursors are not used, the useof organic solvents or plastic containers during grinding or other processing stepsmay introduce carbon. Early claims of successful low-level aliovalent substitution on the Li sites of LiFePO4, resulting in greatly enhanced conductivities andelectrochemical performance, may have been a fortuitous consequence of well-distributed electronically conductive impurities such as carbon and metal-richphosphides [162–166]. Recent studies of the defect chemistry of LiFePO4 showthat substitution of multivalent ions on the Li site is very limited, and alwaysaccompanied by lithium vacancies, so that no mixed valency for iron occurs. Earlier computational modeling of the defect, dopant, and Li transportproperties of LiFePO4  indicates that substitution of multivalent ions on Lior Fe sites (other than divalent ions on the latter) is not energetically favored. It waspredicted that the most likely type of defect is the Li-Fe anti-site pair, in which Li+ions are located on Fe2+ sites and are balanced by an equal number of Fe2+ ions onLi sites. Recent work, however, shows that there is a marked asymmetry betweenthe number of Fe ions on Li sites and vice versa [169–171]. Very few lithium atomscan be accommodated on iron sites. More commonly, Fe ions on Li sites areaccompanied by a small number of vacancies, to form [Li1À2xFex]FePO4. Thepresence of relatively immobile multivalent ions on Li sites interferes with fast Lidiffusion, since LiFePO4 is essentially a one-dimensional ion conductor [172–174].Likewise, a large number of anti-site defects are likely to impact electrochemicalperformance adversely [175, 176] as is seen in Refs. [169–171]. At any rate, it isapparent that near room temperature, only a relatively small concentration ofvacancies or interstitial defects is possible. Carbon coatings, although convenient for the reasons stated above, are notabsolutely necessary to assure good electrochemical performance , as long asparticle sizes are kept small and particle size distributions are narrow.Nanostructuring reduces diffusion distances and ameliorates the effects of lowelectronic conductivity, allowing full discharge at even moderate to high rates. Subtlechanges in the discharge characteristics of LiFePO4 samples occur as particle sizeis decreased, most notably, a stronger dependence of voltage upon composition(x in LixFePO4) close to the end-of-charge and end-of-discharge, implying solid-solution behavior [178, 179]. Other researchers have observed XRD, neutron diffrac-tion, and electrochemical evidence of a small degree of lithium non-stoichiometryin larger LixFePO4 particles at both composition extremes [180, 181], asillustrated in Fig. 2.9. The existence of a small degree of non-stoichiometry (and thus mixed valencestates for iron) may explain why this system is electroactive, given that both endmembers have such poor electronic conductivity. It should be noted, however,that kinetic effects, surface impurities, and the presence of defects [179, 182–184]also inﬂuence the shape of the Li/LiFePO4 discharge proﬁle. This makes it hard to
2 Battery Cathodes 25 x in LixMPO4 0.0 0.2 0.4 0.6 0.8 1.0 FePO4 5 Li1–βFePO4 LiαFePO4 LiαFePO4 Li1–βFePO4 4 Voltage/V LiFePO4 3 2 Single phase region Single phase region Two phase region 1 0 50 100 150 200 Capacity/mAhg–1Fig. 2.9 Scheme of the discharge processes of LixFePO4, showing solid-solution behavior close tox = 0 and x = 1 (Used with permission from Ref. ) 350 D 300 Temperature (°C) 250 H+D D+T 200 150 H T 100 H+T 50 0 0 0.2 0.4 0.6 0.8 1 FePO4 x in LixFePO4 LiFePO4Fig. 2.10 Phase diagram of the LixPO4 system, where T, H, and D denote triphylite, heterosite,and disordered (but not amorphous) phases, respectively (Used with permission from Ref. )determine what the exact compositional ranges of solid-solution behavior are atroom temperature from the electrochemical data alone. Complications from theeffects of strain also make the interpretation of diffraction data difﬁcult. Experiments conducted on heated LiFePO4/FePO4 mixtures of varyingconcentrations [185, 186] show that solid solutions form from 0 x 1 inLixFePO4 at elevated temperatures, however. A representative phase diagram isshown in Fig. 2.10. The solubility limits of lithium in heterosite and vacancies in
26 M.M. Doeff 200 nm 2.120 nm a/c =2.05 (FePO ) 4.341 nm 4 4.00 nm a c a c a/c =2.19 (Li FePO4) 4.420 nm 2.015 nmFig. 2.11 Left: TEM image showing a partially delithiated crystal with the global compositionLi0.5FePO4, showing domains of LiFePO4 and FePO4 aligned along the c-axis. Right: High-resolution TEM image with Fourier transforms of the boxed areas, identifying the two phases(Used with permission from Ref. )triphylite are approximated in the ﬁgure, because of the uncertainties outlinedabove. Additionally, due to slow kinetics, the exact temperature boundaries arenot known, explaining the differences observed by various researchers. Dependingupon the initial concentration, and details of the crystal sizes and morphologies,metastable lithium-deﬁcient phases can persist for remarkably long times aftercooling . The mechanism of the LiFePO4/FePO4 electrochemical reaction has beendescribed using a shrinking core model , as depicted in Fig. 2.9. Duringdischarge, lithium initially inserts into FePO4 to form the solid-solution LiaFePO4phase, where a is close to 0. Upon further passage of current, a shell of a lithium-richmaterial (Li1ÀbFePO4) is produced on the surface, over a core of LiaFePO4. As thereaction continues to progress, the shell grows at the expense of the core, and theinterface between the two phases shrinks, until complete conversion to Li1ÀbFePO4occurs. Further lithiation produces LiFePO4 at the end-of-discharge. The entireprocess is reversed upon charge. The anisotropy of lithium diffusion in LiFePO4[172–174], however, complicates the interpretation of the shrinking core model.A transmission electron microscopy (TEM) study of partially delithiated large plate-like particles  show that ordered domains of FePO4 and LiFePO4 alternate inthe ac plane, separated by narrow disordered (but not amorphous) regions, wherelithium mobility is enhanced. The phase transformation proceeds in the direction ofthe a-axis at dislocation lines that run parallel to the c-axis, consistent with one-dimensional Li+ diffusion in the b-direction (Fig. 2.11). This somewhat resembles an
2 Battery Cathodes 27early “mosaic” model proposed by Andersson et al. as an alternative to the shrinkingcore model . These observations also suggest that the best rate performance canbe achieved with particles that are thin in the direction of Li diffusion (b-axis), butthat nanostructuring in other directions may not be required. In another recent study  using high-resolution electron energy loss spectros-copy (EELS) on a chemically prepared sample, a different distribution of the twophases in a partially delithiated particle was observed. In this case, LiFePO4 waspresent only at the edges with FePO4 located in the interior (but not on surfaces of theac planes) of plate-like particles signiﬁcantly smaller than those studied in Ref.. This is consistent with a progressive emptying or ﬁlling of Li channelsoriented along the b-axis, with the front between the two phases moving perpendic-ular to the ac plane. No disordered regions at the phase boundaries were detected,however. This lack of evidence for solid-solution behavior argues againsta shrinking core mechanism, which requires that at least a small degree ofnon-stoichiometry exist in the system. Variations in particle sizes and morphologies, as well as in the concentration ofdefects, may well inﬂuence the progression of the delithiation reaction during chemi-cal oxidation and explain these differing results. In electrochemical cells with com-posite electrodes, the reaction may nucleate preferentially at sites where contact withconductive carbon additives or coatings and the electrolyte solution is the closest,leading to a different pattern of phase distributions than is seen in the chemicallydelithiated samples, where nucleation can occur at numerous sites simultaneously. Inpartially delithiated LixFePO4 samples recovered from electrochemical cells, nomixed-phase nanoparticles were observed, leading the researchers to surmise thatthe reaction front propagates much more rapidly than nucleation . A recentkinetic study also indicates that the LiFePO4/FePO4 transformation is controlled bya phase-boundary reaction . However, newly discovered evidence ofintercrystallite ionic transport, leading to a redox reaction between delithiated andlithiated particles and subsequent equilibration  complicates the interpretation ofthese results. Moreover, areas of composite electrodes with poor electronic connectiv-ity may be electrochemically inactive, leading to islands of unreacted LiFePO4. In thatcase, all of the lithium will be extracted from LiFePO4 in better connected areas, andmixtures of FePO4 and LiFePO4 will be observed, as in Ref. . While the actual mechanism of the LiFePO4/FePO4 transformation remainsa subject of debate, it seems clear that the shrinking core model does not apply tothe primary particles themselves. The model may, however, still be applicable ona larger scale, for example, to the secondary particles comprised of agglomerates. Over the past decade, better control of synthesis parameters, the use ofconductive coatings, and nanostructuring have transformed LiFePO4 froma poorly performing material to one of the most attractive cathodes for Li-ionbatteries. LiFePO4 appears to be particularly well suited to high-power applicationsincluding power tools and vehicle propulsion. A recent study shows that extraordi-narily high charge and discharge currents can be sustained in cells designed so thata modiﬁed LiFePO4 limits rate . (While these devices are not practical for real-world use, they serve to demonstrate the intrinsic rate capability of LiFePO4
28 M.M. Doeffwithout interference from mass transfer limitations in other cell components).There have been reports [196, 197] of iron dissolution in LiPF6-containingelectrolytes leading to capacity fading at elevated temperatures (analogous to theproblems observed with manganese oxide spinels), although this may be due tothe presence of iron-containing surface impurities such as Fe2P rather than to theLiFePO4 itself. The thermal properties of the LiFePO4/FePO4 system area particularly attractive feature, leading to enhanced safety (LFP, Table 2.2).Upon heating, FePO4 produced by charging LiFePO4 transforms to the thermody-namically favored trigonal form (a-quartz structure). While this reaction is irre-versible and leads to loss of capacity, it progresses without evolution of oxygen. This is in contrast to transition metal oxides, all of which lose oxygen tosome degree at high states-of-charge. This makes this cathode especially appealingfor traction applications, where safety is paramount. Because LiFePO4 is less dense than the layered oxides or spinels (the crystallo-graphic density is 3.6 g/cm3 compared to about 5 g/cm2 for the oxides), and thepotential versus lithium is lower, the energy density is less than that of the oxides(Table 2.2). The speciﬁc energy, in contrast, is competitive with LMO (Table 2.1),but for many applications, the energy per unit volume matters more than per weight.The discharge potential of the isostructural LiMnPO4 is about 0.5 V versus Li/Li+higher than that of LiFePO4 , which increases the speciﬁc energy by about15%. Unfortunately, this material is even less dense than LiFePO4 (3.4 g/cm3), andthe conductivity appears to be several orders of magnitude lower [200, 201].Synthetic procedures used to produce nanoparticulate LiMnPO4 and variantsinclude sol-gel, precipitation, combustion techniques, spray pyrolysis, and hydro-thermal or solvothermal (polyol process) methods [176, 202–208]. For samplescalcined in air for the sake of convenience, a fair amount of carbon is generallyadded after synthesis to offset the low conductivity. Coating can also be achievedvia incorporation of carbonaceous precursors or elemental carbon during heattreatment under inert atmosphere, as with LiFePO4. Electrochemical performanceimproves as the average primary particle size decreases . Partial Mg substitu-tion on the Mn site is also beneﬁcial [208, 210–212]. This effect has been attributedto stabilization against strain associated with the Jahn–Teller distortion of Mn3+ions in the delithiated phase, as well as decreased volume changes upon cycling.The best results reported so far have been for solvothermally prepared powders(polyol process) embedded in a carbon matrix . Still, the rate capability ofLiMnPO4 is not as impressive as that of LiFePO4, and many of the strategiesemployed to improve the electrochemistry (Mg substitution, addition of largeamounts of carbon, nanostructuring) reduce the already fairly small energy densityadvantage. The disappointing performance has been variously attributed to poortransport properties in either the bulk LiMnPO4 or MnPO4 phases, the instability ofthe MnPO4 phase itself, or surface effects [201, 214, 215]. While the voltage proﬁleof LiMnPO4 is ﬂat during charge and discharge, indicating a two-phase process,evidence of solid-solution behavior near the MnPO4 limit has been observed .As with the LiFePO4/FePO4 system, the non stoichiometry may enable the
2 Battery Cathodes 29electrochemical activity. However, no solid-solution behavior near the LiMnPO4end of the phase diagram has yet been detected. Although the performance characteristics of the LiMnPO4/MnPO4 system mayimprove with further work, one troubling aspect of this electrode is its thermalinstability in the charged state. Unlike LiFePO4, MnPO4 evolves oxygen gas uponheating to 200 C and decomposes to form Mn2P2O7 [217, 218]. The instability ofMnPO4 is probably related to the strong Jahn–Teller distortion of the Mn3+ ion.LiMnPO4 is therefore less attractive than LiFePO4 in terms of safety, and does nothave better performance characteristics than the metal oxides. Charging is alsosomewhat problematic, because high over-potentials are required due to the kineticlimitations. Thus, it seems unlikely that this cathode material will prove useful fortraction batteries in the near term, although other applications may be feasible. Phospho-olivine compounds containing Co or Ni also exist. LiCoPO4 exhibitselectrochemical activity at about 4.8 V versus Li/Li+ [219, 220]. LiNiPO4 ispredicted to discharge at about 5.1 V in a lithium cell, but appears to be nearlycompletely inactive . Neither of these is likely to be used as cathodes forlithium-ion batteries in the near term in part because of the very high voltagesneeded to charge the materials, which present a number of practical problems. Solid solutions containing a mixture of transition metals can be prepared overa wide composition range . Li[MnyFe1Ày]PO4 compounds exhibit two plateausin the discharge proﬁle at about 4.1 and 3.45 V versus Li/Li+ with their relativemagnitudes proportional to the amounts of Mn and Fe, respectively . Ingeneral, for y 0.8, the mixed metal phospho-olivines appear to undergo morefacile electrochemical reactions than the pure end-member phase, LiMnPO4 [215,222]. A study of the delithiation reactions of these phases  suggested that thesystem is single phase when x 1Ày, but biphasic over the 4.1 V plateau(corresponding to the Mn2+/Mn3+ redox couple). A later synchrotron diffractionstudy  showed two two-phase regions roughly coinciding with the twoplateaus and a narrow solid-solution region between x = 0.55 and 0.67 forLixMn0.6Fe0.4PO4, corresponding to the steeply sloping portion of the dischargeproﬁle between the plateaus. Other mixed transition metal phospho-olivines have been prepared containingNi and Co  and Fe, Mn, and Co [225–227]. In the case of the Li[NiyCo1Ày]PO4, only one plateau was observed at 4.8 V, corresponding to the Co2+/Co3+ redoxcouple. The only effect of the Ni substitution is to reduce the overall capacity,demonstrating the poor electro-activity of Ni in the phospho-olivine structure. Inlithium cells containing LiMn1/3Fe1/3Co1/3PO4, on the other hand, three distinctelectrochemical features are observed, corresponding to redox processes ofthe three types of transition metals (Fig. 2.12). Interestingly, the reaction appearsto be single phase over the entire composition range, 0 x 1 in LiMn1/3Fe1/3Co1/3PO4, and the redox potentials of the Fe2+/Fe3+ and Co2+/Co3+ couples are slightlyshifted compared to the corresponding LiMPO4 electrodes containing only onemetal. The manganese redox processes appear to be more sluggish than those ofiron and cobalt, and at higher discharge rates, the electrochemical feature at 4.1 Vdisappears. Tailoring of the voltage proﬁle by incorporating multiple metals in the
30 M.M. DoeffFig. 2.12 Charge and 5discharge of a Li/LiMn1/3Fe1/3Co1/3PO4 cell, showing threedistinct plateauscorresponding to the redox ofCo (4.8 V), Mn (4.1 V), and Fe 4 Voltage (V)(3.45 V) (Used withpermission from Refs.[225–227]) 3 2 0 40 80 120 160 Capacity (mAh g–1)olivine structure may have practical use as a state-of-charge indicator for vehicularbatteries (acting much like the gas gauge in conventional combustion engineautomobiles).Other Phosphates and Poly-anionic CompoundsThere are many other transition metal-containing poly-anionic compounds withstructures amenable to lithium insertion processes. Among these are numerousmaterials with the Nasicon structure (Nasicon stands for sodium superionicconductor and originally referred to Na1+xZr2P3ÀySiyO12 compounds ).These have the general formula AxM2(XO4)3, where A is an alkali metal oralkaline earth, M is a transition metal or combination of transition metals, andX is P, As, Si, or S or a combination of these. M is octahedrally coordinated byoxygen, and X is tetrahedrally coordinated. All corners of the XO4 tetrahedra areshared with MO6 octahedra and vice versa; these link to form open channels inwhich the alkali or alkaline earth ions are located. There are also closely relatedthree-dimensional framework structures with differing arrangements of corner-sharing polyhedra and distributions of alkali metal cations, such as the monoclinicLi3Fe2(PO4)3 shown in Fig. 2.13. Transport of alkali metal ions through the tunnels in Nasicons can be extremelyrapid, particularly at elevated temperatures, although the electronic conductivities arelow. For these reasons, these materials were originally proposed for use as solid ionicconductors (e.g., to replace b00 alumina in high temperature Na/S batteries). In spite oftheir low electronic conductivities, researchers recognized that Nasicon structures withredox-active transition metals and related three-dimensional framework compoundscould function as electrode materials as early as the late 1980s [229–231] and numer-ous materials were investigated [232, 233]. In many cases, the electrochemical
2 Battery Cathodes 31Fig. 2.13 The structure ofmonoclinic Li3Fe2(PO4)3looking down the unique axis.P is located in the bluetetrahedra, and Fe in thegreen octahedra. Li ions arerepresented as spheresproperties are unsuitable for Li-ion batteries. For example, Li cannot be extracted frommonoclinic Li3Fe2(PO4)3, only inserted, and the discharge occurs at a rather lowvoltage (2.8 V versus Li/Li+). In contrast, up to two lithiums per formula unit can beextracted reversibly from monoclinic Li3V2(PO4)3, corresponding to a capacity ofabout 130 mAh/g at an average potential of 3.8 V [234–236]. Complex multiphasicbehavior is exhibited upon redox, resulting in multiple plateaus in the discharge proﬁle.In spite of signiﬁcant volume changes upon lithium insertion and extraction, thematerial shows very good cycling behavior. Fluorophosphates are relatively rare, but have recently been studied for Li-ionapplications. The lithium in LiVPO4F [237–239] can be extracted reversibly ata potential of about 4.2 V versus Li/Li+. Interestingly, lithium can also be inserted atabout 1.8 V. Thus, a graphite-free lithium-ion battery can be built, using LiVPO4Fas both the anode and the cathode! Na3V2(PO4)2F3 , Na2FePO4F , andLiFePO4F [242, 243] have also been investigated. The ﬁrst two compounds wereused as-is in electrochemical cells, and underwent ion exchange in situ. Althoughthese cathodes eventually stabilize when used in lithium metal cell conﬁgurationsand the cycling behavior is good, the presence of sodium in full cells with graphiteanodes may disrupt the SEI layer and is therefore undesirable. Thus, thesecompounds will have to be ion-exchanged prior to use. In the case of LiFePO4F,the investigators saw some evidence that a small amount of lithium could beextracted (with concomitant oxidation of Fe3+ to Fe4+), but the main electrochemi-cal reaction was insertion of lithium and reduction of Fe3+ to Fe2+. Other electroactive phosphorus-containing compounds include iron(III)hydroxyl phosphates with lipscombite or tavorite structures [244, 245], b- and e-VOPO4 [246–248], and LiVP2O7 . Although the Nasicons, three-dimensionalframework structures, and the aforementioned phosphates and diphosphates allhave interesting electrochemical properties, most are not competitive with LiFePO4or the commercialized metal oxides for a variety of reasons. The iron-containingmaterials generally discharge at too low a voltage for use in Li-ion battery
32 M.M. DoeffFig. 2.14 Views of a b-polymorph of Li2MSiO4 looking down the a-axis (left), the b-axis(middle), and the c-axis (right). MO4 (yellow) and SiO4 (pink) tetrahedra alternate and connectto form layers through which lithium ions (green spheres) can diffuseconﬁgurations and many have fairly low capacities. Some would need to belithiated prior to use. The vanadium-containing materials cycle well, and havesufﬁciently high voltages and capacities to ensure high energy density, but raiseconcerns about toxicity and environmental impact. Interest has also recently been directed toward a family of silicates with thegeneral composition Li2MSiO4, where M is a divalent cation such as Fe2+, Mn2+,and Co2+ or a combination of these [250–257]. The chemical formula implies that itmay be possible to extract two Li ions per transition metal unit, giving a very hightheoretical speciﬁc capacity of about 330 mAh/g. These materials adopt structuresin which Li, Si, and the transition metal ions all occupy tetrahedral sites ina distorted close-packed oxygen array. The particular polymorph obtained dependsupon the nature of the transition metal as well as the temperature and method ofpreparation. In the b-polymorphs (low-temperature forms), the tetrahedra shareonly corners, and all point in the same direction. In g-polymorphs (high temperatureforms), triads of tetrahedra are arranged so that the central one points in the oppositedirection and shares edges with the two outer tetrahedra. Numerous tetrahedralstructures exist, with different ordering of the ions and varying degrees of distor-tion. Several different views of an electroactive b-polymorph (space group Pmn21)are shown in Fig. 2.14, which illustrates its quasi-layered nature. Accurate structuredetermination of these phases is complicated by the presence of impurities in manypreparations and variations in synthetic procedures, which may lead to subtlestructural differences [256, 258]. About one Li+ per formula unit can be extracted from Li2FeSiO4 in electrochemicalcells at low current densities and at 60 C [250, 251]. The initial extraction takes placeat about 3.1 V versus Li/Li+, but subsequent discharges and charges occur at 2.8 V.This indicates that a structural change takes place, the exact nature of which is notentirely clear. After this initial change, however, relatively good cycling is observed,with an overall capacity of about 130 mAh/g (corresponding to somewhat less than 1Li+ per Li2FeSiO4). There is no experimental evidence that more than one Li+ can beextracted, and ﬁrst principle calculations indicate that it is not possible to do so atpotentials compatible with conventional organic liquid electrolytes .
2 Battery Cathodes 33 The differences between the potentials at which the ﬁrst and second lithium ionscan be extracted are much smaller when M=Mn, Co, or Ni in Li2MSiO4 than when it isFe, however. As with the olivine system, the redox potentials for Li2MnSiO4 electro-chemical processes (at least for extraction of the ﬁrst lithium) are expected to be withinthe oxidative stability limits of organic electrolytes, while those of Li2CoSiO4 andLi2NiSiO4 are probably not. However the electrochemical behavior of Li2MnSiO4appears to be much worse than that of Li2FeSiO4 [251, 254]. Belharaouk et al. were able to achieve initial discharge capacities of about 135 mAh/g at room temper-ature, over a wide voltage range, by using carbon-coated submicron-sized particles,but this is still far less than predicted for complete extraction of all the lithium.Discharge capacities as high as about 250 mAh/g, however, can be obtained whenmixed metal compounds Li2MnxFe1ÀxSiO4 [252, 256] are used as cathodes in lithiumcells. Unfortunately, the quality of the energy obtained is poor because the voltageproﬁles are steeply sloping over a range of about 4.5–1.0 V versus Li/Li+. At such lowpotentials, relatively little power can be obtained from the electrode. The extremeslope may be partly due to the severe kinetic and electronic limitations of thematerials, leading to large over-potentials in lithium cells. If so, a combination ofthe carbon-coating and nanostructuring strategies used to improve the olivines mayameliorate the poor voltage characteristics and lead to new cathodes with nearlydouble the energy currently available.Conversion ElectrodesA different class of electrode materials is based not upon insertion processes but onthe displacement reactions of binary metal compounds [260, 261] (Eq. 2.4): nLiþ þ neÀ þ Mnþ Xm $ M þ nLiXm=n ðX ¼ O, F, N, SÞ (2.4) Conversion electrodes have long been used in primary systems (e.g., Li/CFxbatteries), but have only been proposed for use in rechargeable devices recently,when it was recognized that the reactions could be made reversible fornanoparticulate materials. While the speciﬁc capacities can be enormous, the volt-age characteristics make most of these electrodes more suitable for use as anodesrather than as cathodes. A notable exception seems to be that of metal ﬂuorides,which are electroactive anywhere from 2 to 4 V versus Li/Li+, depending on theidentity of the metal, with speciﬁc capacities as high as 600 mAh/g. It is typical ofconversion electrodes to exhibit signiﬁcant hysteresis upon recharge, which may beintrinsic to the materials and processes. The mechanisms of conversion reactions arecomplex and involve bond breaking and considerable rearrangement, unlike that ofinsertion electrodes. The reassembly of the original phase upon recharge does notnecessarily involve the same kinetic pathways and intermediates as the productionof the elemental metal and LiF during discharge. Thus, it may not be possible to
34 M.M. Doeffremove the hysteresis entirely either by engineering of devices or by improving thematerial properties to ensure faster rate capability. This property has an adverseeffect on the round-trip efﬁciencies, and may make conversion electrodes unsuitablefor Li-ion batteries unless a solution can be found to this problem.Future DirectionsBecause none of the cathode materials discussed above are ideal for every applica-tion, the search for new insertion electrodes continues. Batteries are relativelysimple devices, but the simultaneous requirements for high energy density, longcycle life, safety, and low cost impose stringent restrictions upon the choicesavailable for cathode materials. The highly successful example of LiFePO4 hasdirected researchers toward the exploration of other poly-anionic compounds thatmay share its excellent thermal stability at high states of charge. It is now evidentthat nanostructuring and/or conductive coatings can overcome kinetic and elec-tronic limitations, allowing materials that would once have been thought of asunsuitable for electrodes to be considered. Changes in the phase behavior ofnanoparticulate materials (in comparison to the conventionally sized powders)can render compounds electroactive that, in bulk form, appear to be unpromisingdue to their insulating nature. The shortened diffusion distances for lithium innanoparticles may enable high rate capability in powders that appear to have severerate limitations when micron-sized or larger. While this allows the menu ofpotential cathodes to be greatly expanded, the concept of “going nano” should beapproached with caution. It is most successful when it is applied to materials thatundergo redox well within the electrolyte stability range, such as with LiFePO4.The increased surface area of nanoparticulate powders compared to conventionallysized materials exacerbates any tendency toward irreversible reaction withelectrolytes. In addition to the very serious safety concerns this raises, the paradox-ical result may be to lower rate capability due to the increased presence of resistivereaction layers on cathode particle surfaces ! Nano-sizing may also adverselyimpact practical speciﬁc energies because processing into electrodes becomes moredifﬁcult. It is often necessary, for example, to add more carbon to the compositecathode to ensure good electrical connectivity, but this contributes dead weight.High surface area particles also do not pack well, leading to decreases in the tapdensities and lower energy densities. Ensuring that nanoparticles are regularlyshaped rather than irregularly can ameliorate these tendencies, however .Another potentially useful approach is to synthesize mesoporous materials in which the particles are micron-sized but contain pores of controlled sizes anddistributions so as to maximize contact between the electrolyte and active material.This effectively shortens diffusion distances, while minimizing the tap densityeffects and maintaining the ease of electrode processing. The use of nano metric or very thin coatings on cathode particle surfaces toimprove the electronic conductivity of a material, to decrease dissolution, suppress